Andrew Rusinko Int. Journal of Engineering Research and Applications ISSN : 2248-9622, Vol. 4, Issue 3( Version 1), March 2014, pp.172-180

RESEARCH ARTICLE

www.ijera.com

OPEN ACCESS

Feigen’s Phenomenon in Terms of the Synthetic Theory Andrew Rusinko Obuda University, Népszínház St. 8, Budapest, Hungary, H-1081

Abstract The paper concerns with the analytic description of Feigen’s results on plastic straining under combined loading. The model is developed in terms of the synthetic theory of irrecoverable deformation. Criterion to establish when Feigen’s phenomenon can be observed is proposed. It is worthwhile to note that the synthetic theory requires no special additional assumptions, or generalizations to model Feigen’s experiment. Keywords: Feigen’s phenomenon, plastic deformation, combined loading, synthetic theory of irrecoverable deformation

I. Introduction Feigen’s experimental results (Feigen, M., 1954) are of crucial importance to obtain further insight into mechanisms of plastic deforming. Despite the fact that this phenomenon dates back to the 1950s of the twentieth century, its modeling has not been completely solved yet. Consider Feigen’s experiment consisting in the following loading regime: (i) a specimen plastically deforms in a complex stress state, tension and torsion (Fig. 1a); (ii) the torsional component decreases and the tension increases, (Fig. 1b). The loading path (ABC, AC>AB ) is shown in Fig. 2. Feigen reports an unexpected phenomenon is observed. The torsional plastic deformation ( S ) accumulated in the initial combined loading decreases during the torsional unloading, S 0 along BC portion: the specimen is plastically “untwisting”. According to classical ideas, a plastic strain developed in active loading remains unchangeable during the succeeding unloading. This phenomenon can be explained by the fact that, along portion BC, plastic shifts develop within such slip systems that give negative increment in torsional strain thereby resulting in the plastic untwisting of specimen. At the same time, the fraction of grains, which produced positive torsional strains along portion AB, remains hardened along BC. The aim of the paper is to model Feigen’s experiments in terms of the synthetic theory of recoverable deformation. Another goal of the study is to establish a criterion for predicting the condition when the phenomenon is manifested. It is worth noting that the synthetic theory needs no additional assumptions or generalizations; its classical statement is readily applicable to the analytical description of Feigen’s results. In contrast, for example, Mazilu, P. (1985) tried to explain this phenomenon by assuming the existence of certain hypoelastic deformations (Lehmann, Th., 1962) accompanying the elasto-plastic one. The research presented here may be of interest for the studies dealing with a wide variety of engineering mechanics (Mirsalimov and Veliyev (2013); Szekeres (2012); Kharchenko and Sobkowski (2005); Zabłocka et al. (2012); Malinin, V. (2011)). It is clear that Feigen’s phenomenon can not be modeled in terms of classical flow plasticity theories (for an extensive review, see Rees, 1987). If we take, for example, flow plasticity theory with isotropic hardening rule, it will relate plastic strain tensor components increment ( dijS ) to stress deviator tensor components ( ij ) as d ijS ij C 0 d 0 ,

(1.1)

where 0 is the second invariant of stress tensor and C 0 is C 0

1 2 0

1 1 , Gt G

(1.2)

where G is elastic shear modulus and Gt d 0 3d 0 ( 0 is the second invariant of strain tensor). Condition

Gt G implies that C 0 0 . www.ijera.com

172 | P a g e

Andrew Rusinko Int. Journal of Engineering Research and Applications ISSN : 2248-9622, Vol. 4, Issue 3( Version 1), March 2014, pp.172-180

www.ijera.com

For the case of biaxial loading (tension + torsion), Eq. (1.1) give d S C 0 d 0 , d S C 0 d 0 .

(1.3)

In terms of the flow theory with isotropic hardening, plastic deformation is assumed to develop if d0 0 . If to suggest that d0 0 along portion BC ( 0 and 0 ), then Eq. (1.3) gives positive increments in both S and S components. For the case d0 0 , we have d S d S 0 . Both results contradict Feigen’s experiment reporting that d S 0 .

II. Mathematical apparatus: the synthetic theory of irrecoverable deformation. The synthetic theory, which concerns with small strains of work-hardening metals, incorporates the elements of flow plasticity theory (Sanders, 1954) and slip concept (Budiansky, 1949). The fundamentals of the synthetic theory are put forth in details in Rusinko’s works (2009, 2011). (i) The synthetic theory belongs to two-level models. Similarly to the Budiansky slip concept, the synthetic theory has a micro- and a macro-level. For the macrolevel we take as the elementary volume of the body, , which is considered as point in the mathematical sense. The given volume, , consists of a large quantity of volumes, 0 (the micro-level), each being an element of the continuous, capable of deforming under the applied forces. Accordingly to Budiansky, it is assumed that the stress state in every volume 0 is the same as that in the volume . Plastic deformation in the microvolume 0 (grain) is assumed as slip of one part of 0 in relation to another. Therefore, in contrast to the even distribution of the stress above microvolumes 0, the plastic deformation (or plastic slip) depends on the orientation of the slip system relative to the direction of the acting forces. It is assumed that the quantity of 0 is so great (theoretically it tends to infinity) that every possible orientation of slip systems exists in volume . The total deformation of is determined as the sum of the components of deformations generated within volumes 0. Lichatchev et al. (1993) give the substantiation of the sizes of microvolumes 0. (ii) The establishment of stress~strain relationships on microlevel takes place in the three-dimensional subspace, R3, of the Ilyushin five-dimensional stress deviator space, R5, where a loading is presented by stress vector, S R3 , whose components are S1 3 2 S xx , S2 S xx

2 2 S yy , S3 2 S xz ,

(2.1) where S ij are the stress deviator tensor components. The length of the vector S is related to the second invariant of stress deviator tensor ( J 2 ) as S 2 3J 2 . (iii) New yield criterion is introduced, which coincides with nor Tresca’s, no von-Mises’s one in R5. At the same time, its trace in R 3 gives the von-Mises yield criterion: S12 S22 S32 SS2 ,

S S 2 3 S

(2.2)

where S is the yield strength of material in uniaxial tension. Through each point on the sphere we draw a tangent plane. So, the yield surface can be thought of the inner envelope of equidistant planes. The position of plane in R 3 is defined by the following two quantities (Fig. 3): a) Unit vector m(m1 , m2 , m3 ) normal to the plane:

m1 cos cos , m2 sin cos , m3 sin ,

(2.3) 3 where α and β are spherical angles giving the orientation of m in R (Rusinko, 2009). For simplicity, we consider only planes tangential to yield/loading surface in R 3 and those tangential to the yield/loading surface in R 5 are ignored. b) The distance from the origin of coordinates to the plane, hm . The condition that a plane is located on the endpoint of stress vector is expressed as (2.4) hm S m . (iv) According to Sanders, to establish a hardening rule, we extend the provision that a surface is constructed as an inner envelope of planes to the case of loading as well. During loading, the vector S displaces on its endpoint a set of planes from their initial position, i.e. from sphere (2.2). Each plane moves without changing its

www.ijera.com

173 | P a g e

Andrew Rusinko Int. Journal of Engineering Research and Applications ISSN : 2248-9622, Vol. 4, Issue 3( Version 1), March 2014, pp.172-180

www.ijera.com

orientation. As a result, the loading surface – an inner envelope of planes – has a form as shown in Fig. 4. It consists of - a cone whose lateral surface is formed by the boundary planes reached by the S and - the part of sphere (2.2), which is the inner envelope of stationary planes. (v) Each tangent plane corresponds to an appropriate slip system, and the displacement of the plane on the endpoint of stress vector symbolizes the development of plastic microdeformation within the slip system. Plastic microstrain modeled by the displacement of one plane is assumed to be a vector normal to the plane (see Fig. 3). It is easy to see that the distance to a plane gives the degree of the hardening of material. Indeed, the greater hm , the greater stress vector is needed to reach the plane, i.e. to induce plastic shift within the corresponding slip system. Further, we introduce an average measure of plastic strain developed within a slip system (i.e. for one plane), termed as plastic strain intensity ( m ), as follows 2 2 if hm S m (plane is reached by S) 1 hm SS m (2.5) r if hm S m (plane is not reached by S) 0 where r is the constant of material, r MPa 2 . It must be noted that the product S m is the resolve stress acting within a slip system. Further, it is easy to see that the greater hm , the greater distance is traveled by the plane on the endpoint of stress vector, i.e. the greater plastic deformation develops within the corresponding slip system. (vi) The macroplastic deformation, expressed via plastic strain vector components ( ekS ), is calculated as the sum of non-zero m (Rusinko, 2009, 2011): e S de S mmdV , or ekS m mk dV , dV cos d d , k 1, 2,3 .

(2.6)

The components ek from Eq. (2.6) can be converted to the strain deviator tensor components ( eij ) as e1 3 2exx , e2 exx

2 2e yy , e3 2exz

(2.7)

It must be noted that, in terms of the synthetic theory, both loading and deformation are expressed via vectors: S and e S , respectively. It is clear that vector algebra is much easier than tensor analysis. One more point that deserves attention is that vector components Si have the same rights in the criterion (2.2); it is not the case if the von-Mises yield criterion is expressed via, e.g., stress deviator tensor components:

12

2 S xx2 S yy S zz2 2 S xy2 S yz2 S xz2

2 3J 2 .

III. Isotropy postulate in terms of the synthetic theory According to Ilyushin (1963), isotropy postulate reads that if the stress path in R 3 is rotated in stress deviator space, then the corresponding strain path is rotated by the same amount (this postulate is valid for only von-Mises’s medium). Consider an arbitrary loading path in R 3 as shown in Fig. 5. Let the corresponding strain vector be e , which makes angle η with the stress vector S . Now, we rotate the loading path by a certain angle, δ. To demonstrate the fulfillment of the isotropy postulate, we rotate the coordinate system by the same angle δ. Within the rotated coordinate system, we obtain an analog of the previous loading and, therefore, it is easy to conclude that the angle between vectors e and S must be the same as in the initial case. It is clear that the value of strain strongly depends on the inner geometry of the loading path, but the rotation of loading path as a rigid figure does not affect the relation between vectors e and S at any point of loading path.

IV. Feigen’s phenomenon in terms of synthetic theory Relying upon isotropy postulate, we can model Feigen’s phenomenon. We consider the following case: (i) an initial biaxial loading is proportional, i.e. the loading path of the stress vector S is a straight line and (ii) after the loading an infinitesimal orthogonal additional loading is applied ( dS S ). It is clear that such a loading regime falls within the scope of Feigen’s experiment due to the additional loading gives an increase in tension and decrease in torsion. Let the vector S make angle with S1 -axis. Let us introduce a new system of www.ijera.com

174 | P a g e

www.ijera.com

coordinates ( S1 ' S2 ' S3 ' ) by rotating the initial system by the angle so that the stress vector is along the S1 ' axis. In fact, we obtain an analog of two-segment loading, uniaxial tension and additional torsion. Consequently, according to isotropy postulate, techniques developed in Rusinko’s previous works (2009, 2011) can be readily used. In terms of the rotated coordinate system, the stress vector for the initial portion of loading has the only nonzero component: S1 ' 2 3 x ' , S2 ' 0 S3 ' 0 , S SS . (4.1) On the base of Eqs. (2.3)-(2.5), the distance to plane and strain intensity are hm ' S1 ' m1 ' 2 3 x 'cos 'cos ' ,

(4.2)

2 2 x ' cos2 'cos2 ' 2S , (4.3) 3r where angles ' and ' are measured within S1 ' S2 ' S3 ' coordinate system in the same way as within the original system. The only non-zero component of plastic strain vector e S in S1 ' S2 ' S3 ' coordinate system is (by analogy with calculations from Rusinko’s works (2009, 2011)) m '

e1S '

1 1

m ' m1 ' dV

' '

2 3r

' cos2 'cos2 ' 2S cos 'cos 2 'd ' d ' , 2

x

1 1

(4.4)

where

cos 1 '

b , cos '

cos 1 b ,

b

S . x '

(4.5)

By integrating (4.4) over domain (4.5) we obtain

e1S '

42S b , 3r

b

1 1 b2 b2

2

1 0 .

,

(4.6)

Due to the action of dS , which is analogous to additional torsion ( d xz ' ) within S1 ' S2 ' S3 ' coordinate system, the strain intensity acquires the following increment rd m ' 2hm ' dhm ' , (4.7) where dhm ' hm ' hm ' 2 sin ' d xz ' ,

(4.8)

hm ' 2 3 x 'cos 'cos ' 2 sin ' d xz ' .

(4.9)

where hm ' stands for the distance to planes under the action of S dS vector:

As follows from the analysis of two segment orthogonal loading (Rusinko, 2009), plastic strain vector increment components, de1S ' and de3S ' , are calculated as

de ' S 1

d

m

' m1 ' dV

4 x ' d xz ' 3r

' '

de ' S 3

d

m

' m3 ' dV

4 x ' d xz '

' '

3r

1 1

cos

2

'cos3 'sin 'd ' d ' ,

(4.10)

1 0

1 1

cos 'cos

2

'sin 2 'd ' d ' ,

(4.11)

1 0

Comparison of Eqs. (4.10) and (4.11) to Eq. (4.4) – ' -domain is 0,1 and 1 , 1 , respectively – shows that the set of planes being at the endpoint of S vector is two times less than that due to the action of S dS . Integrating in (4.10) and (4.11) yields de1S '

2S 3r x '

b d xz ' ,

www.ijera.com

b

1 1 arccos b 1 b2 1 2b , 2 b b

(4.12)

175 | P a g e

Andrew Rusinko Int. Journal of Engineering Research and Applications ISSN : 2248-9622, Vol. 4, Issue 3( Version 1), March 2014, pp.172-180 de3S '

3e1S ' d xz ' . 2 x '

www.ijera.com

(4.13)

The plot of b is shown in Fig. 6. As we can see from the formulae above, the value of strain increments strongly depends on the value of initial loading. The set of planes displaced by the vector S is shown in Fig. 7a. For the case when the loading path of the vector S is a straight line (proportional loading) (i) the normal vectors of displaced planes are symmetric above S1 ' axis, (ii) planes on either side of the S incurs identical displacements. This means that the total plastic strain vector e S , which is calculated as the sum of strain vectors, each of which is normal to the plane displaced by the S , lies along the S1 ' -axis. To model Feigen’s phenomenon, one needs to analyze the sign of e3S vector during additional loading. In Fig. 7b, planes with m3 0 are depicted by solid lines; they give positive increments in e3S caused by an orthogonal increment in stress. For planes depicted by dashed lines m3 0 , and, consequently, they stand with negative signs in the sum for the e3S . It is clear that the sign of e3S depends on the set of ―positive‖ and ―negative‖ planes and the distances they traveled on the endpoint of stress vector. The number of planes displaced by additional vector dS is two times less than under the action of S (Fig. 7b), and this set of the planes contains the same number of planes with negative normals (i.e. normals with negative components on S 3 -axis), while the number of planes with positive normals halves. This fact implies that the slope of the strain vector due to the action of S dS vector is less than that due to the S vector. Feigen’s phenomenon, an negative increment in plastic shear deformation during additional loading dS , is observed when the sum of plastic deformation increments having negative components on S 3 -axis is greater than that having positive components on S 3 -axis. Now, we wish to establish a criterion for occurring of Feigen’s phenomenon. In other words, we need to establish such an angle between stress vector S and S1 -axis, angle in Fig. 8, so that the orthogonal additional loading results in the negative component of de S on S 3 -axis, de3S 0 . By projecting vector de S de1S ' de3S ' on S 3 - axis and using Eqs. (4.12) and (4.13), we obtain de3S de1S 'sin de3S 'cos

(4.14)

Eq. (4.14) at de3S 0 , together with (4.12) and (4.13), gives

tan 0

S 3 S 1

de ' de '

3e1S ' d xz ' 2 x ' 2S 3r x '

b d xz '

3re1S ' . 22S b

(4.15)

If 0 , then de3S 0 , meaning that Feigen’s phenomenon will be observed. This situation is shown in Fig. 8a. For the case 0 (Fig. 8b), we have de3S 0 implying a positive increment in plastic torsional deformation due to dS , which contradicts Feigen’s phenomenon. Therefore, Eq. (4.15) can be treated as a criterion for occurring Feigen’s phenomenon as a function of the parameters of initial loading.

V. Conclusion The present paper has modeled Feigen’s phenomenon in terms of the synthetic theory. A condition for the onset of negative shear plastic strain under the additional loading has been derived. We restrict ourselves to the case when the additional loading is perpendicular to the initial one. It has been shown that parameters of initial loading, the orientation and magnitude of stress vector, considerably affects the behavior of specimen under the second portion of loading.

www.ijera.com

176 | P a g e

www.ijera.com

References [1] [2] [3] [4] [5] [6] [7]

[8] [9] [10] [11] [12] [13] [14] [15]

Batdorf, S., Budiansky, B. (1949). Mathematical theory of plasticity based on the concept of slip. NACA, Technical note, 871 Feigen, M. (1954), Inelastic behavior under combined tension and torsion, 2nd USNCAM, pp. 469-476. Ilyushin, A.A. (1963). Plasticity, Moscow. Kharchenko, Y., Sobkowski, S. (2005) Modelowanie matematyczne procesów rozruchu układów napędowych podnośników budowlanych, Diagnostyka, 35: 37-42. (in Polish) Lehmann, Th. (1962). Zur Besehreibung groBer plastischer Form~nderungen unter Beriicksichtigung der Werkstoffverfestigung, Rheol. Acta 2: 247-254. Lichatchev, V., Malinin, V. (1993). Structural-analytic theory of strength, St. Petersburg (in Russian). Malinin, V. (2011) Structural and analytical criterion of the fragile destruction for matter with macroconcentration tension, J. Fundamental and Applied Problems of Engineering and Technology, 2: 36-42. Mazilu, P. (1985). Decreasing of the Initial Shear Modulus with Increasing Axial Strain Explained by Means of a Plastic-Hypoelastic Model, Acta Mechanica 55: 93-115. Mirsalimov, V., Veliyev, F. (2013) Inverse Problem of Failure Mechanics for a Drawing Die Strengthened with a Holder, Acta Polytechnica Hungarica, 10: 121-138. Rees, D.W.A. (1987). Application of Classical Plasticity Theory to Non-Radial Loading Paths, Proc. R. Soc. Lond. A, 410: 443-475. Rusinko, A., Rusinko, K. (2009). Synthetic theory of irreversible deformation in the context of fundamental bases of plasticity, Int. J. Mech. Mater. 41: 106-120. Rusinko, A., Rusinko, K. (2011). Plasticity and Creep of Metals, Springer, Berlin. Sanders, I. (1954). Plastic stress-strain relations based on linear loading function, 2nd USNCAM, p. 455460. Szekeres, A. (2012) Cross-Coupled Heat and Moisture Transport: Part 1—Theory, Journal of Thermal Stresses, 35: 248-268. Zabłocka, M., Wieczorek, P., Kłysz, S. (2012) Filtration properties of track membranes, Inżynieria Materiałowa, 33: 51-55.

www.ijera.com

177 | P a g e

www.ijera.com

x

S1 a)

x

S2 b)

T1

y

σx

T2

y

T1 z

T2 < T1

z

S1

S2 > S1 Fig. 1 Loading regime in Feigen’s experiment; S denotes stretching force and T does torque

τ B

C A σ Fig. 2 Loading path in σ-τ plane in Feigen’s experiment

Plastic strain vector

S3

S3

m

m Initial position

Yield surface hm

S1

hm

S

S S2

Current position on the endpoint of stress vector

S1

Traveled distance

S2

Fig. 3 Scheme of the displacement of tangent plane

www.ijera.com

178 | P a g e

www.ijera.com

Displaced planes S Boundary plane 3

S

Stationary planes

S1

Loading surface Yield surface: sphere (2.2) Boundary plane

SS

Fig. 4 Loading surface in terms of the synthetic theory

S2 Loading path

e

η

S

δ δ

S2 ' S1

S

e η

S1 ' Fig. 5 On isotropy postulate

Φ(b)

Fig. 6 Function b from Eq. (4.12)

www.ijera.com

b

179 | P a g e

S3

S3 '

a)

m β1

eS

S3

S3 '

S1 '

www.ijera.com

m dS

b) S

S β1

β1 S1

m

SS

m

SS

Fig. 7 Set of planes displaced by vector S (a) and dS (b) in S1 S3 coordinate plane ( 0 ).

d e1 ' de3 0

S3

S

S3 ' a)

de3

dS

S1 '

de1

de

d e3 '

0

S1 d e1 '

de3 0

b)

de3

de dS

S3

S1 '

de1 d e3 '

S

S3 '

γ > γ0 S1

Fig. 8 The sign of de3 in additional loading depending on the angle of initial loading ( ); superscripts ―S ‖ in strain vectors and components are avoided. www.ijera.com

S1 '

180 | P a g e

S1

Read more

Similar to

Popular now

Just for you